Presentation on theme: "Cutting tool materials The selection of cutting tool material and grade is an important factor to consider when planning a successful metal cutting operation."— Presentation transcript:
Cutting tool materials The selection of cutting tool material and grade is an important factor to consider when planning a successful metal cutting operation. A basic knowledge of each cutting tool material and its performance is therefore important so that the correct selection for each application can be made. Considerations include the workpiece material to be machined, the component type and shape, machining conditions and the level of surface quality required for each operation.
Cutting-Tool Materials Tool bits generally made of seven materials –High-speed steel –Cast alloys (such as stellite) –Cemented carbides –Ceramics –Cermets –Cubic Boron Nitride –Polycrystalline Diamond
Cutting Tool Properties Hardness –Cutting tool material must be 1 1/2 times harder than the material it is being used to machine. Capable of maintaining a red hardness during machining operation –Red hardness: ability of cutting tool to maintain sharp cutting edge –Also referred to as hot hardness or hot strength
Wear Resistance –Able to maintain sharpened edge throughout the cutting operation –Same as abrasive resistance. Shock Resistance –Able to take the cutting loads and forces Shape and Configuration –Must be available for use in different sizes and shapes.
Letter symbols specifying the designation of hard cutting materials Hard metals: HW Uncoated hard metal containing primarily tungsten carbide (WC). HT Uncoated hard metal, also called cermet, containing primarily titanium carbides (TIC) or titanium nitrides (TIN) or both. HC Hard metals as above, but coated
High-Speed Steel May contain combinations of tungsten, chromium, vanadium, molybdenum, cobalt. Can take heavy cuts, withstand shock and maintain sharp cutting edge under red heat Generally two types (general purpose) –Molybdenum-base (Group M) –Tungsten-base (Group T) Cobalt added if more red hardness desired
Cast Alloy Usually contain 25% to 35% chromium, 4% to 25% tungsten and 1% to 3% carbon –Remainder cobalt Qualities –High hardness –High resistance to wear –Excellent red-hardness Operate 2 ½ times speed of high-speed steel Weaker and more brittle than high-speed steel
Letter symbols specifying the designation of hard cutting materials Ceramics: CA Oxide ceramics containing primarily aluminium oxide (Al2O3). CM Mixed ceramics containing primarily aluminium oxide (Al2O3) but containing components other than oxides. CN Nitride ceramics containing primarily silicon nitride (Si3N4). CC Ceramics as above, but coated.
Letter symbols specifying the designation of hard cutting materials Diamond: DP Polycrystalline diamond* Boron nitride: BN Cubic boron nitride* *(Polycrystalline diamond and cubic boron nitride are also called superhard cutting materials ).
Cutting tool materials have different combinations of hardness, toughness and wear resistance, and are divided into numerous grades with specific properties. Generally, a cutting tool material that is successful in its application should be: Hard, to resist flank wear and deformation Tough, to resist bulk breakage Non-reactive with the workpiece material Chemically stable, to resist oxidation and diffusion Resistant to sudden thermal changes.
Coated cemented carbide (HC) Coated cemented carbide currently represents 80-90% of all cutting tool inserts. Its success as a tool material is due to its unique combination of wear resistance and toughness, and its ability to be formed in complex shapes. Coated cemented carbide combines cemented carbide with a coating. Together they form a grade which is customized for its application. Coated cemented carbide grades are the first choice for a wide variety of tools and applications.
Coating – CVD Definition and properties: CVD stands for Chemical Vapor Deposition. The CVD coating is generated by chemical reactions at temperatures of 700-1050°C. CVD coatings have high wear resistance and excellent adhesion to cemented carbide. The first CVD coated cemented carbide was the single layer titanium carbide coating (TiC). Alumina coatings (Al2O3) and titanium nitride (TiN) coatings were introduced later. More recently, the modern titanium carbonitride coatings (MT-Ti(C,N) or MT-TiCN, also called MT-CVD) were developed to improve grade properties through their ability to keep the cemented carbide interface intact.
Modern CVD coatings combine MT-Ti(C,N), Al2O3 and TiN. The coating properties have been continuously improved for adhesion, toughness and wear properties through microstructural optimizations and post-treatments. MT-Ti(C,N) - Its hardness provides abrasive wear resistance,resulting in reduced flank wear. CVD-Al2O3 – Chemically inert with low thermal conductivity, making it resistant to crater wear. It also acts as a thermal barrier to improve plastic deformation resistance. CVD-TiN - Improves wear resistance and is used for wear detection. Post-treatments - Improve edge toughness in interrupted cuts and reduce smearing tendencies.
Applications CVD coated grades are the first choice in a wide range of applications where wear resistance is important. Such applications are found in general turning and boring of steel, with crater wear resistance offered by the thick CVD coatings; general turning of stainless steels and for milling grades in ISO P, ISO M, ISO K. For drilling, CVD grades are usually used in the peripheral insert.
Coating – PVD Definition and properties Physical Vapor Deposition (PVD) coatings are formed at relatively low temperatures (400-600°C). The process involves the evaporation of a metal which reacts with, for example, nitrogen to form a hard nitride coating on the cutting tool surface. PVD coatings add wear resistance to a grade due to their hardness. Their compressive stresses also add edge toughness and comb crack resistance.
The main PVD-coating constituents are described below. Modern coatings are combinations of these constituents in sequenced layers and/or lamellar coatings. Lamellar coatings have numerous thin layers,in the nanometer range, which make the coating even harder. PVD-TiN - Titanium nitride was the first PVD coating. It has all-round properties and a golden color. PVD-Ti(C,N) - Titanium carbonitride is harder than TiN and adds flank wear resistance. PVD-(Ti,Al)N - Titanium aluminium nitride has high hardness in combination with oxidation resistance, which improves overall wear resistance. PVD-oxide - Is used for its chemical inertness and enhanced crater wear resistance.
Applications PVD coated grades are recommended for tough, yet sharp, cutting edges, as well as in smearing materials. Such applications are widespread and include all solid end mills and drills, and a majority of grades for grooving, threading and milling. PVD-coated grades are also extensively used for finishing applications and as the central insert grade in drilling.
Cemented carbide Definition and properties Cemented carbide is a powdery metallurgical material; a composite of tungsten carbide (WC) particles and a binder rich in metallic cobalt (Co). Cemented carbides for metal cutting applications consist of more than 80% of hard phase WC. Additional cubic carbonitrides are other important components, especially in gradient sintered grades. The cemented carbide body is formed, either through powder pressing or injection moulding techniques, into a body, which is then sintered to full density.
WC grain size is one of the most important parameters for adjusting the hardness/toughness relationship of a grade; the finer grain size means higher hardness at a given binder phase content. The amount and composition of the Co-rich binder controls the grade’s toughness and resistance to plastic deformation. At equal WC grain size, an increased amount of binder will result in a tougher grade, which is more prone to plastic deformation wear. A binder content that is too low may result in a brittle material. Cubic carbonitrides, also referred to as γ-phase, are generally added to increase hot hardness and to form gradients. Gradients are used to combine improved plastic deformation resistance with edge toughness. Cubic carbonitrides concentrated in the cutting edge improve the hot hardness where it is needed. Beyond the cutting edge, a binder rich in tungsten carbide structure inhibits cracks and chip hammering fractures.
Applications Medium to coarse WC grain size Medium to coarse WC grain sizes provide the cemented carbides with a superior combination of high hot hardness and toughness. These are used in combination with CVD or PVD coatings in grades for all areas. Fine or submicron WC grain size Fine or submicron WC grain sizes are used for sharp cutting edges with a PVD coating to further improve the strength of the sharp edge. They also benefit from a superior resistance to thermal and mechanical cyclic loads. Typical applications are solid carbide drills, solid carbide end mills, parting off and grooving inserts, milling and grades for finishing. Cemented carbide with gradient The beneficial dual property of gradients is successfully applied in combination with CVD coatings in many first choice grades for turning, and parting and grooving in steels and stainless steels.
Uncoated Cemented Carbide (HW) Definition and properties Uncoated cemented carbide grades represent a very small proportion of the total assortment. These grades are either straight WC/Co or have a high volume of cubic carbonitrides. Applications Typical applications are machining of HRSA (heat resistant super alloys) or titanium alloys and turning hardened materials at low speed. The wear rate of uncoated cemented carbide grades is rapid yet controlled, with a self- sharpening action.
Cermet (CT) Definition and properties A cermet is a cemented carbide with titanium based hard particles. The name cermet combines the words ceramic and metal. Originally, cermets were composites of TiC and nickel. Modern cermets are nickel-free and have a designed structure of titanium carbonitride Ti(C,N) core particles, a second hard phase of (Ti,Nb,W)(C,N) and a W-rich cobalt binder. Ti(C,N) adds wear resistance to the grade, the second hard phase increases the plastic deformation resistance, and the amount of cobalt controls the toughness. In comparison to cemented carbide, cermet has improved wear resistance and reduced smearing tendencies. On the other hand, it also has lower compressive strength and inferior thermal shock resistance. Cermets can also be PVD coated for improved wear resistance.
Applications Cermet grades are used in smearing applications where built-up edge is a problem. Its self-sharpening wear pattern keeps cutting forces low even after long periods in cut. In finishing operations, this enables a long tool life and close tolerances, and results in shiny surfaces. Typical applications are finishing in stainless steels, nodular cast irons, low carbon steels and ferritic steels. Cermets can also be applied for trouble shooting in all ferrous materials. Hints: Use low feed and depth of cut. Change the insert edge when flank wear reaches 0.3 mm. Avoid thermal cracks and fractures by machining without coolant.
Ceramic (CA, CM, CN, CC) Definition and properties All ceramic cutting tools have excellent wear resistance at high cutting speeds. There are a range of ceramic grades available for a variety of applications. Oxide ceramics are aluminium oxide based (Al2O3), with added zirconia (ZrO2) for crack inhibition. This generates a material that is chemically very stable, but which lacks thermal shock resistance. (1) Mixed ceramics are particle reinforced through the addition of cubic carbides or carbonitrides (TiC, Ti(C,N)). This improves toughness and thermal conductivity.
(2) Whisker-reinforced ceramics use silicon carbide whiskers (SiCw) to dramatically increase toughness and enable the use of coolant. Whisker-reinforced ceramics are ideal for machining Ni-based alloys. (3) Silicon nitride ceramics (Si3N4) represent another group of ceramic materials. Their elongated crystals form a self-reinforced material with high toughness. Silicon nitride grades are successful in grey cast iron, but a lack of chemical stability limits their use in other workpiece materials. Sialon (SiAlON) grades combine the strength of a self-reinforced silicon nitride network with enhanced chemical stability. Sialon grades are ideal for machining heat resistant super alloys (HRSA).
CC620 Oxide ceramic for high speed finishing of grey cast iron in stable and dry conditions. CC6050 Mixed ceramic for light, continuous finishing in hardened materials. CC650 Mixed ceramic for high speed finishing of grey cast irons and hardened materials, and for semi-finishing operations in HRSA with low toughness demands. CC670 Whisker ceramic with excellent toughness for turning, grooving and milling of Ni- based alloys. Can also be used for hard part turning in unfavorable conditions. CC6190 Silicon nitride grade for rough to finish turning and high speed dry milling of cast iron, perlitic nodular CC6090 cast irons and hardened cast irons. CC6090 Coated silicon nitride grade for light roughing to finish turning of cast iron. GC1690 Sialon grade for optimized performance when turning pre-machined HRSA in stable conditions. CC6060 Predictable wear due to good notch wear resistance. CC6065 Particle reinforced Sialon for turning operations in HRSA that demand tough inserts.
Polycrystalline cubic boron nitride, CBN (BN) Definition and properties Polycrystalline cubic boron nitride, CBN, is a material with excellent hot hardness that can be used at very high cutting speeds. It also exhibits good toughness and thermal shock resistance. Modern CBN grades are ceramic composites with a CBN content of 40-65%. The ceramic binder adds wear resistance to the CBN, which is otherwise prone to chemical wear. Another group of grades are the high content CBN grades, with 85% to almost 100% CBN. These grades may have a metallic binder to improve their toughness.
CBN is brazed onto a cemented carbide carrier to form an insert. The Safe-Lok™ technology further enhances the bondage of CBN cutting tips on negative inserts. Applications CBN grades are largely used for finish turning of hardened steels, with a hardness over 45 HRc. Above 55 HRc, CBN is the only cutting tool which can replace traditionally used grinding methods. Softer steels, below 45 HRc, contain a higher amount of ferrite, which has a negative effect on the wear resistance of CBN. CBN can also be used for high speed roughing of grey cast irons in both turning and milling operations.
CB7015 PVD coated CBN grade with ceramic binder for continuous turning, and light interrupted cuts in hardened steels. CB7025 CBN grade with ceramic binder for interrupted cuts and high toughness demands when turning hardened steels. CB7050 High content CBN grade with metallic binder for heavy interrupted cuts in hardened steels and for finishing grey cast iron. PVD coated.hardness demands when turning hardened steels.
Definition and properties PCD is a composite of diamond particles sintered together with a metallic binder. Diamond is the hardest, and therefore the most abrasion resistant, of all materials. As a cutting tool, it has good wear resistance but it lacks chemical stability at high temperatures and dissolves easily in iron. Polycrystalline diamond, PCD (DP) CD10 PCD grade for finishing and semi-finishing of non-ferrous and non-metallic materials in turning and milling.
Wear on cutting edges To understand the advantages and limitations of each material, it is important to have some knowledge of the different wear mechanisms to which cutting tools are subjected. Abrasive Flank wear The most common type of wear and the preferred wear type, as it offers predictable and stable tool life. Flank wear occurs due to abrasion, caused by hard constituents in the workpiece material.
Chemical Crater wear Crater wear is localized to the rake side of the insert. It is due to a chemical reaction between the workpiece material and the cutting tool and is amplified by cutting speed. Excessive crater wear weakens the cutting edge and may lead to fracture. Adhesive Built-up edge (BUE) This wear type is caused by pressure welding of the chip to the insert. It is most common when machining sticky materials, such as low carbon steel, stainless steel and aluminium. Low cutting speed increases the formation of built-up edge.
Adhesive Notch wear Insert wear characterized by excessive localized damage on both the rake face and flank of the insert at the depth of cut line. Caused by adhesion (pressure welding of chips) and a deformation hardened surface. A common wear type when machining stainless steels and HRSA. Thermal Plastic deformation Plastic deformation takes place when the tool material is softened. This occurs when the cutting temperature is too high for a certain grade. In general, harder grades and thicker coatings improve resistance to plastic deformation wear.
Thermal Thermal cracks When the temperature at the cutting edge changes rapidly from hot to cold, multiple cracks may appear perpendicular to the cutting edge. Thermal cracks are related to interrupted cuts, common in milling operations, and are aggravated by the use of coolant. Mechanic Edge chipping/breakage Chipping or breakage is the result of an overload of mechanical tensile stresses. These stresses can be due to a number of reasons, such as chip hammering, a depth of cut or feed that is too high, sand inclusions in the workpiece material, built-up edge, vibrations or excessive wear on the insert.